Effective enhancement of mechanical properties <i>via</i> H/F substitution in 3D cyanide hybrid perovskites.
Ji, Luan-Ying; Zhou, Jun-Si; Liu, Shu-Yi; Qin, Yan; Lv, Hui-Peng; Chen, Xiao-Gang; Chemical communications (Cambridge, England) 61 (2025) 13165–13168; doi:10.1039/d5cc03229f

data_7134870
_publ_section_title
;
 Effective enhancement of mechanical properties <i>via</i> H/F
 substitution in 3D cyanide hybrid perovskites.
;
_journal_issue                   70
_journal_name_full               'Chemical communications (Cambridge, England)'
_journal_page_first              13165
_journal_page_last               13168
_journal_paper_doi               10.1039/d5cc03229f
_journal_volume                  61
_journal_year                    2025
_chemical_formula_moiety         'C12 Fe2 K2 N12, 4(C2 H7 F N)'
_chemical_formula_sum            'C20 H28 F4 Fe2 K2 N16'
_chemical_formula_weight         758.48
_space_group_crystal_system      cubic
_space_group_IT_number           225
_space_group_name_Hall           '-F 4 2 3'
_space_group_name_H-M_alt        'F m -3 m'
_atom_sites_solution_hydrogens   geom
_audit_creation_method           SHELXL-2018/3
_audit_update_record
;
2023-12-09 deposited with the CCDC.	2025-07-24 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   11.8392(4)
_cell_length_b                   11.8392(4)
_cell_length_c                   11.8392(4)
_cell_measurement_reflns_used    281
_cell_measurement_temperature    423(2)
_cell_measurement_theta_max      73.0290
_cell_measurement_theta_min      10.6050
_cell_volume                     1659.46(10)
_computing_cell_refinement       'CrysAlisPro 1.171.42.79a (Rigaku OD, 2022)'
_computing_data_collection       'CrysAlisPro 1.171.42.79a (Rigaku OD, 2022)'
_computing_data_reduction        'CrysAlisPro 1.171.42.79a (Rigaku OD, 2022)'
_computing_structure_refinement  'SHELXL-2018/3 (Sheldrick, 2018)'
_computing_structure_solution    'SHELXT 2018/2 (Sheldrick, 2018)'
_diffrn_ambient_temperature      423(2)
_diffrn_detector_area_resol_mean 10.0000
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 0.983
_diffrn_measurement_device_type  'XtaLAB Synergy R, DW system, HyPix'
_diffrn_measurement_method       '\w scans'
_diffrn_radiation_type           CuK\a
_diffrn_radiation_wavelength     1.54184
_diffrn_reflns_av_R_equivalents  0.0108
_diffrn_reflns_av_unetI/netI     0.0087
_diffrn_reflns_Laue_measured_fraction_full 1.000
_diffrn_reflns_Laue_measured_fraction_max 0.983
_diffrn_reflns_limit_h_max       10
_diffrn_reflns_limit_h_min       -14
_diffrn_reflns_limit_k_max       4
_diffrn_reflns_limit_k_min       -13
_diffrn_reflns_limit_l_max       10
_diffrn_reflns_limit_l_min       -13
_diffrn_reflns_number            436
_diffrn_reflns_point_group_measured_fraction_full 1.000
_diffrn_reflns_point_group_measured_fraction_max 0.983
_diffrn_reflns_theta_full        67.684
_diffrn_reflns_theta_max         74.499
_diffrn_reflns_theta_min         6.476
_diffrn_source                   'Rotating-anode X-ray tube'
_exptl_absorpt_coefficient_mu    9.808
_exptl_absorpt_correction_T_max  1.00000
_exptl_absorpt_correction_T_min  0.64133
_exptl_absorpt_correction_type   multi-scan
_exptl_crystal_colour            'dull reddish brown'
_exptl_crystal_density_diffrn    1.518
_exptl_crystal_description       block
_exptl_crystal_F_000             772
_refine_diff_density_max         0.524
_refine_diff_density_min         -0.998
_refine_diff_density_rms         0.111
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.154
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     43
_refine_ls_number_reflns         119
_refine_ls_number_restraints     62
_refine_ls_restrained_S_all      0.858
_refine_ls_R_factor_all          0.0797
_refine_ls_R_factor_gt           0.0795
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.2200P)^2^] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.2112
_refine_ls_wR_factor_ref         0.2131
_reflns_Friedel_coverage         0.000
_reflns_number_gt                115
_reflns_number_total             119
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            d5cc03229f2.cif
_cod_data_source_block           lmz_fyakfecn6_423k_auto
_cod_depositor_comments
'Adding full bibliography for 7134868--7134871.cif.'
_cod_original_cell_volume        1659.46(17)
_cod_database_code               7134870
_shelx_shelxl_version_number     2018/3
_shelx_res_checksum              99237
_shelx_hkl_checksum              43056